IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 47, NO. 11, NOVEMBER 2000

2161

A Physical Model for Hole Direct Tunneling Current in P+ Poly-Gate PMOSFETs with Ultrathin Gate Oxides Kuo-Nan Yang, Huan-Tsung Huang, Student Member, IEEE, Ming-Chin Chang, Che-Min Chu, Yuh-Shu Chen, Ming-Jer Chen, Senior Member, IEEE, Yeou-Ming Lin, Mo-Chiun Yu, Simon M. Jang, Douglas C. H. Yu, and M. S. Liang

Abstract—A model of the hole direct tunneling gate current accounting for heavy and light hole’s subbands in the quantized inversion layer is built explicitly. This model comprises four key physical parameters: inversion layer charge density, hole impact frequency on SiO2 /Si interface, WKB transmission probability, and reflection correction factor. With the effective hole mass = 0 51 for parabolic dispersion relationship in the oxide, experimental reproduction without any parameter adjustment is consistently achieved in p+ poly-gate pMOSFETs with 1.23, 1.85, and 2.16 nm gate oxide thicknesses. The proposed model can thereby serve as a promising characterization means of direct tunnel oxides. In particular, it is calculated that the secondary subbands and beyond, although occupying few holes, indeed contribute substantially to the direct tunneling conduction due to effective lower barrier heights, and are prevailing over the first subbands for reducing oxide field down below 1 MV/cm.

I. INTRODUCTION

T

HE MOSFET gate oxide thickness is rapidly approaching the direct tunneling limit that ultimately leads to intolerably increased standby power [1] and/or impractical applications [2]. Thus, accurate characterization and modeling of ultrathin oxides in the direct tunneling regime is essential and crucial. A series of models have recently been published concerning the electron direct tunneling in n poly-gate nMOSFETs: a self-consistent numerical method of solving Schrödinger’s and Poisson’s equations [1] and computationally efficient models [3], [4]. The latter can provide more transparent understandings since it is made up of four key physical parameters: accumulation or inversion layer charge density, electron impact frequency on interface, WKB transmission probability, and specially, the reflection correction factor [3], [4]. As to another complementary devices, namely, p poly-gate pMOSFETs, the hole direct tunneling under channel inversion condition was found to dominate over valence electron direct tunneling [5], followed by

Manuscript received March 8, 2000. This work was supported by the National Science Council under the Contract NSC88-2215-E-009-047. The review of this paper was arranged by Editor C.-Y. Lu. K.-N. Yang, H.-T. Huang, M.-J. Chang, C.-M. Chu, Y.-S. Chen, and M.-J Chen are with the Reliability Physics Laboratory and Institute of Electronics, National Chiao-Tung University, Hsinchu 300, Taiwan, R.O.C. (e-mail: [email protected]) Y.-M. Lin, M.-C. Yu, S. M. Jang, D. C. H. Yu, and M. S. Liang are with the R&D Department, Taiwan Semiconductor Manufacturing Company, Hsinchu 300, Taiwan, R.O.C. Publisher Item Identifier S 0018-9383(00)09621-0.

more evidences [6], [7]. In this paper, we present a model of the hole direct tunneling current featuring the above four similar physical parameters. This model can serve as a promising means of sensitively characterizing direct tunnel oxides and can enable in-depth understandings of the roles of the subbands in the quantized inversion layer. II. CHARACTERIZATION AND PARAMETER EXTRACTION The p poly-gate pMOSFETs were fabricated by a 0.18m process technology [8] with gate oxides grown in diluted wet oxygen ambient to three different thicknesses. The gate 100 m . Accurate determidimension was drawn to 100 is strongly demanded. nation of ultrathin oxide thickness Three techniques in terms of high resolution TEM(HRTEM), polysilicon depletion and quantum mechanics corrected capacitance–voltage (C–V) [9]–[11], and direct tunneling (DT) I–V [3] were adopted as shown in Fig. 1, through which consistent results were achieved as compared in Fig. 2. Fig. 1(a) just shows highly-localized HRTEM cross section while the variation across the wafer is depicted in Fig. 2 in terms of a bar. Our C–V data in Fig. 1(b) was measured in parallel mode with 1-MHz AC frequency. QM corrected C–V fitting based on van Dort’s model for surface quantization [9], [10] was carried out . In particular, the singular point problem to extract physical was eliminated encountered around the flat-band voltage by adopting a modified version [11]. In Fig. 1(b), C–V fitting for nm is limited to nondistorted range, 0.6 V 0.6 V, where the tunneling current effect or others can be neglected. C–V fitting in Fig. 1(b) also produced the p polysilcm and the icon dopant concentration cm , effective channel dopant concentration all being found to be consistent with the SIMS doping profile. In Fig. 1(c), the devices were biased in channel accumulation (positive gate voltage) with source, drain, and -well tied to ground, was get in advance by means and the oxide field strength of the well-known C–V integration technique. With the effective for Franz-type dispersion relaelectron mass tionship in the oxide, the conduction electron DT I–V fitting in , 1.85, and 2.16 nm from three Fig. 1(c) extracted samples. Note that as all data go closer to the straight line with the unity slope in Fig. 2, more confidence for DT I–V extracted , as well as its subsequent applications in consistently calculating the DT hole current, can all be ensured.

0018–9383/00$10.00 © 2000 IEEE

2162

IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 47, NO. 11, NOVEMBER 2000

(a) (a)

(b) (b)

(c)

I

' I T

Fig. 3. (a) Measured hole direct tunneling current ( ) and valence electron tunneling current ( ) of three different under 0 . (b) The carrier separation configuration and (c) band diagram representation are schematically drawn.

V < V

I

'I

(c) Fig. 1. (a) HRTEM images of three pMOSFET gate stacks. T values extracted from the canvases correspond to 2.25, 1.89, and 1.32 nm, respectively. (b) The oxide thickness extraction using C–V method was based on van Dort’s model [9] and successive researchers [10], [11]. Best fitting produces T of 2.0, 1.75, and 1.3 nm, respectively. (c) I–V fitting to find T . T values extracted by electron direct tunneling model [3], including quantization effect in accumulation layer under , are 2.16, 1.85, and 1.23 nm, respectively.

V >V

Fig. 2. Comparing

T

extracted from several techniques.

With source, drain, and n-well tied to ground, the source/drain ), bulk current ( ), and gate current ( ) meacurrent ( sured in inversion are plotted in Fig. 3(a) versus gate voltage ( ). The corresponding carrier separation configuration and the band diagram representation are schematically drawn in Fig. 3(b) and (c), respectively. It can be identified that the hole direct tunneling is responsible for source/drain current while the valence electron direct tunneling constitutes bulk current. It is seen from Fig. 3 that the hole direct tunneling dominates over the valence-band electron direct tunneling in gate voltage of 0 V to certain crossover point, which is consistent with [5]–[7]; however, the magnitude of this crossover gate voltage increases with decreasing oxide thickness, a phenomenon not mentioned before. A specific criterion of 1 A/cm at gate voltage of 1 V sets an ultimate limit of slightly thicker than 1.23 nm, again consistent with [2]. The impact of hole direct tunneling on normal device operation can be found in Fig. 4, revealing that the hole direct tunneling from inverted channel can reverse the polarity of the linear drain current. The similar drain current degradations for the n-channel counterpart have been reported

YANG et al.: HOLE DIRECT TUNNELING CURRENT IN P

POLY-GATE PMOSFETS

2163

electron direct tunneling in [3]. Hole current density contributed by th subband with energy to can be written as (1) where

=

Fig. 4. Measured output I –V characteristics with W=L 10 m/50 m and T = 1:23 nm. I reverses its polarity at small jV j due to direct hole tunneling.

elemental charge; impact frequency of hole’s wave packet on interface; inversion layer charge density per unit area and magnitude of associated with th subband; transmission probability through layer. as the classical turning point at the th subband Denoting as the velocity of edge and wave packet (2) Triangle-like electrostatic potential is a good approximation . Using Sommerfeld-Wilson’s quantization rule, we are for direction able to get quantized energy along -direction or in reciprocal space

For inversion charge increment

(3) Fig. 5. Physical picture of valence hole quantized phenomenon along h100i direction. G (E ) indicates density of states relative to hole’s energy. F (E ) represents Fermi–Dirac distribution function of hole and E means the quantized extremity energy of the j th subband.

previously [12], [13]. The impact of hole DT as outlined in Fig. 4 is one of the primary motivations of the underlying study. To clarify the essential mechanisms, however, the work focuses on the case of tying source and drain to a common potential. III. PHYSICAL MODEL The two valence bands (heavy and light band), which are de( point), have the form of warped spheres; generate at method concerning degenerate perturbation therefore, the is necessary for the valence band [14]:

In (3), density of states per unit area for two-dimensional hole , is equal to and Fermi–Dirac distrigas (2DHG), associated with valence holes is bution function . is the quasi–Fermi level and is Boltzmann’s constant. Under the inversion condition, it is easy . means the to build that signifies that on the potential drop on the p -poly gate, and n-well. Considering the poly-depletion effect, we know that can be expressed as . Note that the values are obtained by the C–V integraof oxide field strength tion technique so that the surface potential, , can be comis equal to . Here puted directly. Thus, is the potential difference between ) and valence band ( ) in the the quasi–Fermi level ( charge neutrality region of n-well. can be modeled by Following [3], (4) where

Fig. 5 schematically shows the physical picture of the valence-band hole tunneling from the silicon inversion layer. In direction Fig. 5, a table lists the effective mass ( ) along and density of states mass ( ) of each type of hole as cited in [15]. The direct tunneling hole current from each subbands can be formulated in analogy with the mathematical treatment of

is the barrier height of tunneling hole with total energy at cathode side or p -poly gate/ interface, and is

2164

IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 47, NO. 11, NOVEMBER 2000

that at anode side or /n-well interface. and . In our work, the barrier height is 4.7 eV for both heavy and light hole. The total energy, , consists of the transversal and longitudinal energies

where is the transversal mass. On the other hand, is a justified factor concerning wavefunction’s reflection phenomenon interfaces as discussed in [3] and [4], as occurring at follows:

Fig. 6. Simulated results (lines) and experimental data (symbols) for pMOSFET direct tunneling hole current of three different T under 0 V. can be related to by means of the C–V integration technique.

V

where and are the group velocities of the holes incident and leaving the oxide, respectively. direction The group velocity of hole with energy along interfaces is independent of within the th subband at with the following expression:

E

V

2161

A Physical Model for Hole Direct Tunneling Current in P+ Poly-Gate PMOSFETs with Ultrathin Gate Oxides Kuo-Nan Yang, Huan-Tsung Huang, Student Member, IEEE, Ming-Chin Chang, Che-Min Chu, Yuh-Shu Chen, Ming-Jer Chen, Senior Member, IEEE, Yeou-Ming Lin, Mo-Chiun Yu, Simon M. Jang, Douglas C. H. Yu, and M. S. Liang

Abstract—A model of the hole direct tunneling gate current accounting for heavy and light hole’s subbands in the quantized inversion layer is built explicitly. This model comprises four key physical parameters: inversion layer charge density, hole impact frequency on SiO2 /Si interface, WKB transmission probability, and reflection correction factor. With the effective hole mass = 0 51 for parabolic dispersion relationship in the oxide, experimental reproduction without any parameter adjustment is consistently achieved in p+ poly-gate pMOSFETs with 1.23, 1.85, and 2.16 nm gate oxide thicknesses. The proposed model can thereby serve as a promising characterization means of direct tunnel oxides. In particular, it is calculated that the secondary subbands and beyond, although occupying few holes, indeed contribute substantially to the direct tunneling conduction due to effective lower barrier heights, and are prevailing over the first subbands for reducing oxide field down below 1 MV/cm.

I. INTRODUCTION

T

HE MOSFET gate oxide thickness is rapidly approaching the direct tunneling limit that ultimately leads to intolerably increased standby power [1] and/or impractical applications [2]. Thus, accurate characterization and modeling of ultrathin oxides in the direct tunneling regime is essential and crucial. A series of models have recently been published concerning the electron direct tunneling in n poly-gate nMOSFETs: a self-consistent numerical method of solving Schrödinger’s and Poisson’s equations [1] and computationally efficient models [3], [4]. The latter can provide more transparent understandings since it is made up of four key physical parameters: accumulation or inversion layer charge density, electron impact frequency on interface, WKB transmission probability, and specially, the reflection correction factor [3], [4]. As to another complementary devices, namely, p poly-gate pMOSFETs, the hole direct tunneling under channel inversion condition was found to dominate over valence electron direct tunneling [5], followed by

Manuscript received March 8, 2000. This work was supported by the National Science Council under the Contract NSC88-2215-E-009-047. The review of this paper was arranged by Editor C.-Y. Lu. K.-N. Yang, H.-T. Huang, M.-J. Chang, C.-M. Chu, Y.-S. Chen, and M.-J Chen are with the Reliability Physics Laboratory and Institute of Electronics, National Chiao-Tung University, Hsinchu 300, Taiwan, R.O.C. (e-mail: [email protected]) Y.-M. Lin, M.-C. Yu, S. M. Jang, D. C. H. Yu, and M. S. Liang are with the R&D Department, Taiwan Semiconductor Manufacturing Company, Hsinchu 300, Taiwan, R.O.C. Publisher Item Identifier S 0018-9383(00)09621-0.

more evidences [6], [7]. In this paper, we present a model of the hole direct tunneling current featuring the above four similar physical parameters. This model can serve as a promising means of sensitively characterizing direct tunnel oxides and can enable in-depth understandings of the roles of the subbands in the quantized inversion layer. II. CHARACTERIZATION AND PARAMETER EXTRACTION The p poly-gate pMOSFETs were fabricated by a 0.18m process technology [8] with gate oxides grown in diluted wet oxygen ambient to three different thicknesses. The gate 100 m . Accurate determidimension was drawn to 100 is strongly demanded. nation of ultrathin oxide thickness Three techniques in terms of high resolution TEM(HRTEM), polysilicon depletion and quantum mechanics corrected capacitance–voltage (C–V) [9]–[11], and direct tunneling (DT) I–V [3] were adopted as shown in Fig. 1, through which consistent results were achieved as compared in Fig. 2. Fig. 1(a) just shows highly-localized HRTEM cross section while the variation across the wafer is depicted in Fig. 2 in terms of a bar. Our C–V data in Fig. 1(b) was measured in parallel mode with 1-MHz AC frequency. QM corrected C–V fitting based on van Dort’s model for surface quantization [9], [10] was carried out . In particular, the singular point problem to extract physical was eliminated encountered around the flat-band voltage by adopting a modified version [11]. In Fig. 1(b), C–V fitting for nm is limited to nondistorted range, 0.6 V 0.6 V, where the tunneling current effect or others can be neglected. C–V fitting in Fig. 1(b) also produced the p polysilcm and the icon dopant concentration cm , effective channel dopant concentration all being found to be consistent with the SIMS doping profile. In Fig. 1(c), the devices were biased in channel accumulation (positive gate voltage) with source, drain, and -well tied to ground, was get in advance by means and the oxide field strength of the well-known C–V integration technique. With the effective for Franz-type dispersion relaelectron mass tionship in the oxide, the conduction electron DT I–V fitting in , 1.85, and 2.16 nm from three Fig. 1(c) extracted samples. Note that as all data go closer to the straight line with the unity slope in Fig. 2, more confidence for DT I–V extracted , as well as its subsequent applications in consistently calculating the DT hole current, can all be ensured.

0018–9383/00$10.00 © 2000 IEEE

2162

IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 47, NO. 11, NOVEMBER 2000

(a) (a)

(b) (b)

(c)

I

' I T

Fig. 3. (a) Measured hole direct tunneling current ( ) and valence electron tunneling current ( ) of three different under 0 . (b) The carrier separation configuration and (c) band diagram representation are schematically drawn.

V < V

I

'I

(c) Fig. 1. (a) HRTEM images of three pMOSFET gate stacks. T values extracted from the canvases correspond to 2.25, 1.89, and 1.32 nm, respectively. (b) The oxide thickness extraction using C–V method was based on van Dort’s model [9] and successive researchers [10], [11]. Best fitting produces T of 2.0, 1.75, and 1.3 nm, respectively. (c) I–V fitting to find T . T values extracted by electron direct tunneling model [3], including quantization effect in accumulation layer under , are 2.16, 1.85, and 1.23 nm, respectively.

V >V

Fig. 2. Comparing

T

extracted from several techniques.

With source, drain, and n-well tied to ground, the source/drain ), bulk current ( ), and gate current ( ) meacurrent ( sured in inversion are plotted in Fig. 3(a) versus gate voltage ( ). The corresponding carrier separation configuration and the band diagram representation are schematically drawn in Fig. 3(b) and (c), respectively. It can be identified that the hole direct tunneling is responsible for source/drain current while the valence electron direct tunneling constitutes bulk current. It is seen from Fig. 3 that the hole direct tunneling dominates over the valence-band electron direct tunneling in gate voltage of 0 V to certain crossover point, which is consistent with [5]–[7]; however, the magnitude of this crossover gate voltage increases with decreasing oxide thickness, a phenomenon not mentioned before. A specific criterion of 1 A/cm at gate voltage of 1 V sets an ultimate limit of slightly thicker than 1.23 nm, again consistent with [2]. The impact of hole direct tunneling on normal device operation can be found in Fig. 4, revealing that the hole direct tunneling from inverted channel can reverse the polarity of the linear drain current. The similar drain current degradations for the n-channel counterpart have been reported

YANG et al.: HOLE DIRECT TUNNELING CURRENT IN P

POLY-GATE PMOSFETS

2163

electron direct tunneling in [3]. Hole current density contributed by th subband with energy to can be written as (1) where

=

Fig. 4. Measured output I –V characteristics with W=L 10 m/50 m and T = 1:23 nm. I reverses its polarity at small jV j due to direct hole tunneling.

elemental charge; impact frequency of hole’s wave packet on interface; inversion layer charge density per unit area and magnitude of associated with th subband; transmission probability through layer. as the classical turning point at the th subband Denoting as the velocity of edge and wave packet (2) Triangle-like electrostatic potential is a good approximation . Using Sommerfeld-Wilson’s quantization rule, we are for direction able to get quantized energy along -direction or in reciprocal space

For inversion charge increment

(3) Fig. 5. Physical picture of valence hole quantized phenomenon along h100i direction. G (E ) indicates density of states relative to hole’s energy. F (E ) represents Fermi–Dirac distribution function of hole and E means the quantized extremity energy of the j th subband.

previously [12], [13]. The impact of hole DT as outlined in Fig. 4 is one of the primary motivations of the underlying study. To clarify the essential mechanisms, however, the work focuses on the case of tying source and drain to a common potential. III. PHYSICAL MODEL The two valence bands (heavy and light band), which are de( point), have the form of warped spheres; generate at method concerning degenerate perturbation therefore, the is necessary for the valence band [14]:

In (3), density of states per unit area for two-dimensional hole , is equal to and Fermi–Dirac distrigas (2DHG), associated with valence holes is bution function . is the quasi–Fermi level and is Boltzmann’s constant. Under the inversion condition, it is easy . means the to build that signifies that on the potential drop on the p -poly gate, and n-well. Considering the poly-depletion effect, we know that can be expressed as . Note that the values are obtained by the C–V integraof oxide field strength tion technique so that the surface potential, , can be comis equal to . Here puted directly. Thus, is the potential difference between ) and valence band ( ) in the the quasi–Fermi level ( charge neutrality region of n-well. can be modeled by Following [3], (4) where

Fig. 5 schematically shows the physical picture of the valence-band hole tunneling from the silicon inversion layer. In direction Fig. 5, a table lists the effective mass ( ) along and density of states mass ( ) of each type of hole as cited in [15]. The direct tunneling hole current from each subbands can be formulated in analogy with the mathematical treatment of

is the barrier height of tunneling hole with total energy at cathode side or p -poly gate/ interface, and is

2164

IEEE TRANSACTIONS ON ELECTRON DEVICES, VOL. 47, NO. 11, NOVEMBER 2000

that at anode side or /n-well interface. and . In our work, the barrier height is 4.7 eV for both heavy and light hole. The total energy, , consists of the transversal and longitudinal energies

where is the transversal mass. On the other hand, is a justified factor concerning wavefunction’s reflection phenomenon interfaces as discussed in [3] and [4], as occurring at follows:

Fig. 6. Simulated results (lines) and experimental data (symbols) for pMOSFET direct tunneling hole current of three different T under 0 V. can be related to by means of the C–V integration technique.

V

where and are the group velocities of the holes incident and leaving the oxide, respectively. direction The group velocity of hole with energy along interfaces is independent of within the th subband at with the following expression:

E

V